Surface Preparation for 3M VHB Tape ApplicationsTechnical BulletinSummary
Most substrates are best prepared by cleaning with a 50:50 mixture of isopropyl alcohol (IPA) and water* prior to applying 3M VHB Tapes. Exceptions to this general procedure that may require additional surface preparation include: Heavy Oils: A degreaser or solvent-based cleaner may be required to remove heavy oil or grease from a surface and should be followed by cleaning with IPA/water. Abrasion: Abrading a surface, followed by cleaning with IPA/water, can remove heavy dirt or oxidation and can increase surface area to improve adhesion. Adhesion Promoters: Priming a surface can significantly improve initial and ultimate adhesion to many materials such as plastics and paints. Porous Surfaces: Most porous and fibered materials such as wood, particleboard, concrete etc. need to be sealed to provide a unified surface. Unique Materials: Special surface preparation may be needed for glass and glass-like materials, copper and copper containing metals and plastics or rubber that contain components that migrate (e.g. plasticizers).
To obtain optimum adhesion, the bonding surfaces must be well unified, clean and dry. Typical surface cleaning solvents are IPA/water mixture (rubbing alcohol) or heptane.* (Steps A and B) Bond strength is dependent upon the amount of adhesive-to-surface contact developed. Firm application pressure develops better adhesive contact and helps improve bond strength. (Steps C and D) Generally, this means that the tape should experience at least 15 psi (100 kPa) in roll down or platen pressure. (Sources- page #4) After application, the bond strength will increase as the adhesive flows onto the surface. At room temperature, approximately 50% of the ultimate strength will be achieved after 20 minutes, 90% after 24 hours and 100% after 72 hours. In some cases, bond strength can be increased and ultimate bond strength can be achieved more quickly by exposure of the bond to elevated temperatures (e.g. 150F [66C] for 1 hour).
Step A: Solvent wipe
Step B: Wipe dry
Step C: Apply tape to surface
Step D: Roll finished joint
Typical Bond Build Over Time100 PERCENT OF FULL BONDs s s s s s
q q q
80s q q 40
q ROOM TEMP 0 20 MIN 1 HOUR
s 150F or ABRADE
*Note: These cleaner solutions contain greater than 250 g/l of volatile organic compounds (VOC). Please consult your local Air Quality Regulations to be sure the cleaner is compliant. When using solvents, be sure to follow the manufacturers precautions and directions for use when handling such materials. (1)
Technical BulletinSurface Preparation for 3M VHB Tape ApplicationsHeavy OilsOn surfaces with a light oily film, or other light contamination, the 50:50 IPA/water solution is usually adequate. Where heavy oils or grease are present, a degreasing solvent such as 3M Prep Solvent 70, 3M Citrus Base Cleaner, mineral spirits, naphtha or similar solvents are suggested to cut the oil. This should always be followed with an IPA/water cleaning to help ensure that any residue or film is removed.* Abrading a surface can serve several functions: Remove heavy levels of dirt or oxide from metals or paints (e.g. galvanized steel). Create additional surface area that can increase adhesion. Smooth a surface to obtain more flatness, allowing improved contact area. Abrasion often helps adhesion to paints and plastics. When abrading, it is important for tapes to have a finely abraded surface. Very small scratches in the surface, generated with circular motion rather than straight-line motion, are most desirable. A surface with many micro-scratches in it can have up to 40% additional available surface area, translating to higher ultimate strength and greater initial adhesion. Scotch-Brite Hand Pads (such as 7447 Maroon or Heavy Duty Green) are good for achieving the right level of abrasion. Tools such as a power palm sander will assist on large jobs. Avoid grinding a surface with coarse abrasive materials, since they may create too rough of a texture for the adhesive to adequately flow into the surface. Always clean the surface with the IPA/water solution or additional methods previously described, and be certain that all loose particles are removed prior to bonding. Exceptions to these abrading guidelines are 3M VHB Tapes 4932 and 4952, as they typically perform best on smooth glossy surfaces and abrasion may reduce the bond strength.
Priming a surface can significantly improve initial and ultimate adhesion to many materials such as plastics and paints because of their low surface energy or the additives they may contain. A primer creates a new surface for 3M VHB Tape to adhere to and can also create a layer that may impede the migration of additives that may be present in a material. It is important for the user to determine the suitability of the 3M VHB Tape, the adhesion promoter and the application process. Rough, porous or fibered materials such as wood, particleboard, cement, etc., have an open surface and require sealing to provide a unified surface for tape bonding. Common sealing materials would include paint, varnish or other hard surface coatings. Fast drying 3M Rubber and Vinyl Spray 80 can also be used to unify the surface and improve the tape bond. Glass, stone, ceramic or other siliceous materials are hydrophilic (water-loving) by nature. Normally, the hydrophilic nature makes pressure sensitive adhesive bond durability susceptible to change under high humidity or exposure to moisture. In basic terms, water vapor can undercut the tape bond and interfere with the normal adhesion forces. Silane coupling agents, added to the IPA/water cleaning solution, can help reduce the water-loving tendency of these surfaces and enhance the tape bond in high moisture environments. Copper, brass, and bronze are prone to oxidation even after the 3M VHB Tape is applied. To prevent a weakening of the bond, a lacquer or varnish should be applied to these surfaces. Be sure to test the tape bond to the sealer on a metal surface to verify good adhesion. Flexible PVC (vinyl) contains plasticizers that can migrate into the tape and affect adhesion. There are several 3M VHB Tapes that are formulated to be resistant to plasticizer migration, or 3M Scotch-Grip Plastic Adhesive 2262, thinned, can serve as a barrier to migration. Rubber materials (e.g. EPDM, neoprene) can have low surface energy and may also contain plasticizers and oils. These require the use of an adhesion promoter for stable bond strength. Test for compatibility with flexible PVC and rubber materials by aging bonded samples for a week at 150F (66C) and check for softening of the adhesive, discoloration or reduction in bond strength.
*Note: These cleaner solutions contain greater than 250 g/l of volatile organic compounds (VOC). Please consult your local Air Quality Regulations to be sure the cleaner is compliant. When using solvents, be sure to follow the manufacturers precautions and directions for use when handling such materials. (2)
Technical BulletinSurface Preparation for 3M VHB Tape ApplicationsSuggested PrimersThe table below offers suggested primers and alternative methods that commonly require primers, adhesion promoters or other surface treatments for successful use with 3M VHB Tapes. This list is not intended to be fully comprehensive but may be useful for many applications. It is very important for the user to determine the suitability of the 3M VHB Tape, primer and application process and compliance with local Air Quality Regulations.ConcernSurface must be clean Oxidation after bonding Non-unified or rough surface, moisture High humidity, moisture
SurfaceSteel or Aluminum Copper, Brass, Bronze Concrete, Brick Glass, Stone, Ceramic Tile
Suggested PrimerNone suggested Lacquer or varnish(b) 3M Rubber and Vinyl Spray 80 3M Silane Glass Treatment AP 115 or similar silane coupling agent in IPA/water mixture(b) 3M Rubber and Vinyl Spray 80, 3M Fastbond 30 Contact Adhesive 3M Primer 94 (additional surface preparation may be required) 3M Primer 94, 3M Scotch-Grip Plastic Adhesive 2262(a) 3M Adhesion Promoter N-200J, 3M Scotch-Grip Plastic Adhesive 1099 3M Primer 94, 3M Scotch-Grip Plastic Adhesive 1099 3M Primer 94 3M Adhesion Promoter 111
AlternativesAbrasion may clean surface, 3M Adhesion Promoter 111 for increased adhesion. Architectural grade coatings Concrete sealer, paint 3M Primer 94
Wood (soft, hard particle board, etc.) Plastics: Polyolefin Non-olefin Polyurethane (Molded or Rubber) Rubber: Neoprene, Santoprene EPDM Paints
Weak fiber layer on surface (e.g., low surface strength) Low adhesion Additives, low adhesion Mold release, low adhesion Migrating oils Low adhesion Low adhesion
Urethane paint, varnish Flame treatment, Corona treatment Abrade or 3M VHB Tapes 4932/4952/5925/5952/5962 Abrade and prime 3M Weather Strip Tapes 3M Weather Strip Tapes Abrade or 3M VHB Tapes 4932/4952/5925/5952/5962, or 3M Primer 94, 3M Scotch-Grip Plastic Adhesive 2262 (a), 3M Adhesion Promoter N-200J Abrade or 3M VHB Tapes 4932/4952/5925/5952/5962, or 3M Primer 94, 3M Scotch-Grip Plastic Adhesive 2262 (a), 3M Adhesion Promoter N-200J 3M VHB Tapes 4945 and 4941 (test for migration)
Coil Coated Aluminum
3M Adhesion Promoter 111
Flexible PVC (Vinyl)
3M Scotch-Grip Plastic Adhesive 2262 (a), 3M Rubber and Vinyl Spray 80
Note: These primers contain greater than 250 g/l of volatile organic compounds (VOC). Please contact your local Air Quality Regulations to be sure these primers are compliant. (a)3M Scotch-Grip Plastic Adhesive 2262 contains 196 g/l VOC. (b)See supplier information.
Primer Source and Description
3M Primer 94, 3M Adhesion Promoter 111 and 3M Silane Glass Treatment AP 115 are available through distributors that carry 3M VHB Tapes. 3M Scotch-Grip Plastic Adhesive 2262 must be thinned in acetone or MEK* in a 1:5 or 1:10 ratio (e.g., 1 part Scotch-Grip plastic adhesive 2262 to 5 parts acetone or MEK). The product is available premixed in either acetone or MEK from: PRC DeSoto at (317) 290-1600. 3M Scotch-Grip Plastic Adhesive 2262T, thinned in 10:1 MEK solution or 3M ScotchGrip Plastic Adhesive 2262TA, thinned in 10:1 acetone solution.* When diluted in acetone at this ratio, this material contains 196 g/l VOC.* Diluted 3M Scotch-Grip Plastic Adhesive 1099 must be thinned in acetone* in a 1:3 ratio (e.g., 1 part Scotch-Grip plastic adhesive 1099 to 3 parts acetone). This thinned material contains zero VOCs when diluted in these ratios. 3M Adhesion Promoter N-200J is available from PRC DeSoto at (317) 290-1600. Silane Coupling Agent is also available premixed in a 91:9 IPA/water solution or as a concentrate. A 0.5 wt. % level of silane* adhesion promoter diluted in a 91:9 IPA/water cleaning solution has been found to be sufficient. Suggested Sources for Silane Coupling Agents: Custom-Pak Products, Inc. (262) 251-6180 available premixed in IPA/water Lancaster Synthesis, Inc. (603) 889-3306 available 100% concentrated *Note: Be sure to read and follow silane and solvent manufacturers precautions and directions for use for proper handling and storage information. (3)
Technical BulletinSurface Preparation for 3M VHB Tape ApplicationsRun an Evaluation Because 3M cannot anticipate all of the different possible surfaces and contaminants that may exist, it is imperative that the user conduct an evaluation to determine the suitability of 3M VHB Tapes, surface preparations procedures, and any other processes that may have an influence on the tape or the bonded parts. Likewise, where there are any changes in plastic or paint formulation, or suppliers of these materials, it is advisable to run evaluations to ensure that the change has not influenced the compatibility of the surface with 3M VHB Tapes.
Hand held J-Roller: Rockler Woodworking and Hardware Phone: (800) 279-4441 Specify #39463 www.rockler.com
All statements, technical information and recommendations contained in this document are based upon tests or experience that 3M believes are reliable. However, many factors beyond 3Ms control can affect the use and performance of a 3M product in a particular application, including the conditions under which the product is used and the time and environmental conditions in which the product is expected to perform. Since these factors are uniquely within the users knowledge and control, it is essential that the user evaluate the 3M product to determine whether it is fit for a particular purpose and suitable for the users method of application.
3M warrants for 24 months from the date of manufacture that 3M VHB Tape will be free of defects in material and manufacture. 3M MAKES NO OTHER WARRANTIES, EXPRESS OR IMPLIED, INCLUDING BUT NOT LIMITED TO, ANY IMPLIED WARRANTY OF MERCHANTABILITY OR FITNESS FOR A PARTICULAR PURPOSE. This limited warranty does not cover damage resulting from the use or inability to use 3M VHB Tape due to misuse, workmanship in application, or application or storage not in accordance with 3M recommended procedures.
Limitation of Remedies and Liability
If the 3M VHB Tape is proved to be defective within the warranty period stated above. THE EXCLUSIVE REMEDY, AT 3MS OPTION, SHALL BE TO REFUND THE PURCHASE PRICE OF OR TO REPAIR OR REPLACE THE DEFECTIVE 3M VHB TAPE. 3M shall not otherwise be liable for loss or damages, whether direct, indirect, special, incidental, or consequential, regardless of the legal theory asserted, including negligence, warranty, or strict liability.ISO 9001: 2000
This Industrial Adhesives and Tapes Division product was manufactured under a 3M quality system registered to ISO 9001: 2000 standards.
3Industrial Business Industrial Adhesives and Tapes Division 3M Center, Building 21-1W-10, 900 Bush Avenue St. Paul, MN 55144-1000 800-362-3550 877-369-2923 (fax) www.3M.com/industrialRecycled Paper 40% pre-consumer 10% post-consumerScotch-Brite is a registered trademark of 3M Company. 3M, VHB and Scotch-Grip are trademarks of 3M Company. Printed in U.S.A. 3M 2007 70-0704-8701-5 (4/07)